# Solutions of practice problems_A6.docx

Description
14.5 Below, molecular weight data for a polypropylene material are tabulated. Compute (a) the number-average molecular weight, (b) the weight-average molecular weight, and (c) the degree of polymerization. Molecular Weight Range (g/mol) xi wi 8,000–16,000 0.05 0.02 16,000–24,000 0.16 0.10 24,000–32,000 0.24 0.20 32,000–40,000 0.28 0.30 40,000–48,000 0.20 0.27 48,000–56,000 0.07 0.11 Solution (a) From the tabulated data, we are asked to compute M n , the number-average molecu
Categories
Published

View again

All materials on our website are shared by users. If you have any questions about copyright issues, please report us to resolve them. We are always happy to assist you.
Related Documents
Share
Transcript
14.5  Below, molecular weight data for a polypropylene material are tabulated. Compute (a) the number-average molecular weight, (b) the weight-average molecular weight, and (c) the degree of polymerization.   Molecular Weight Range (g/mol) x  i   w  i    8,000  –  16,000 0.05 0.02 16,000  –  24,000 0.16 0.10 24,000  –  32,000 0.24 0.20 32,000  –  40,000 0.28 0.30 40,000  –  48,000 0.20 0.27 48,000  –  56,000 0.07 0.11 Solution (a) From the tabulated data, we are asked to compute  M n , the number-average molecular weight. This is carried out below. Molecular wt Range Mean  M i    xi    xi M i  8,000-16,000 12,000 0.05 600 16,000-24,000 20,000 0.16 3200 24,000-32,000 28,000 0.24 6720 32,000-40,000 36,000 0.28 10,080 40,000-48,000 44,000 0.20 8800 48,000-56,000 52,000 0.07 3640  ____________________________  M n  =  x i  M  i  =33,040 g/mol  (b) From the tabulated data, we are asked to compute  M w , the weight-average molecular weight. Molecular wt. Range Mean  M  i   w i   w i  M  i  8,000-16,000 12,000 0.02 240 16,000-24,000 20,000 0.10 2000 24,000-32,000 28,000 0.20 5600 32,000-40,000 36,000 0.30 10,800   40,000-48,000 44,000 0.27 11,880 48,000-56,000 52,000 0.11 5720  ___________________________  M w  = w i  M  i  =36,240 g/mol  (c) Now we are asked to compute the degree of polymerization, which is possible using Equation 14.6. For polypropylene, the repeat unit molecular weight is just m  = 3(  A C ) + 6(  A H ) = (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol And  DP  =  M n m =33,040 g/mol42.08 g/mol=785    14.7  Is it possible to have a poly(methyl methacrylate) homopolymer with the following molecular weight data and a of polymerization of 527? Why or why not?   Molecular Weight Range (g/mol) w  i x  i 8,000  –  20,000 0.02 0.05 20,000  –  32,000 0.08 0.15 32,000  –  44,000 0.17 0.21 44,000  –  56,000 0.29 0.28 56,000  –  68,000 0.23 0.18 68,000  –  80,000 0.16 0.10 80,000  –  92,000 0.05 0.03 Solution This problem asks if it is possible to have a poly(methyl methacrylate) homopolymer with the given molecular weight data and a degree of polymerization of 527. The appropriate data are given below along with a computation of the number-average molecular weight. Molecular wt. Range Mean  M  i    x i    x i  M  i  8,000-20,000 14,000 0.05 700 20,000-32,000 26,000 0.15 3900 32,000-44,000 38,000 0.21 7980 44,000-56,000 50,000 0.28 14,000 56,000-68,000 62,000 0.18 11,160 68,000-80,000 74,000 0.10 7400 80,000-92,000 86,000 0.03 2580  _________________________  M n  =  x i  M  i   = 47,720 g/mol  For PMMA, from Table 14.3, each repeat unit has five carbons, eight hydrogens, and two oxygens. Thus, m  = 5(  A C ) + 8(  A H ) + 2(  A O )   = (5)(12.01 g/mol) + (8)(1.008 g/mol) + (2)(16.00 g/mol) = 100.11 g/mol  Now, we will compute the degree of polymerization using Equation 14.6 as  DP   =  M  n m  = 47,720 g/mol100.11 g/mol = 477  Thus, such a homopolymer is   not possible  since the calculated degree of polymerization is 477 (and not 527).

Jul 23, 2017

#### MANE2220-ENGR2220 Course outline Fall 2013.doc

Jul 23, 2017
Search
Similar documents

View more...
Tags

Related Search